JOURNAL OF MATERIALS SCIENCE: MATERIALS IN MEDICINE 12 (2001) 471±478
Hydroxyapatite implants with designed internal
T.-M. G. CHU1
, J. W. HALLORAN2
, S. J. HOLLISTER1
, S. E. FEINBERG3
Department of Biomedical Engineering, University of Michigan, Ann Arbor, MI 48109, USA
Department of Materials Science and Engineering, University of Michigan, Ann Arbor,
MI 48109, USA
Department of Surgery, University of Michigan, Ann Arbor, MI 48109, USA
Porous hydroxyapatite (HA) has been used as a bone graft material in the clinics for decades.
Traditionally, the pores in these HAs are either obtained from the coralline exoskeletal
patterns or from the embedded organic particles in the starting HA powder. Both processes
offer very limited control on the pore structure. A new method for manufacturing porous HA
with designed pore channels has been developed. This method is essentially a lost-mold
technique with negative molds made with Stereolithography and a highly loaded curable HA
suspension as the ceramic carrier. Implants with designed channels and connection patterns
were ®rst generated from a Computer-Aided-Design (CAD) software and Computer
Tomography (CT) data. The negative images of the designs were used to build the molds on
a stereolithography apparatus with epoxy resins. A 40 vol% HA suspension in propoxylated
neopentyl glycol diacrylate (PNPGDA) and iso-bornyl acrylate (IBA) was formulated. HA
suspension was cast into the epoxy molds and cured into solid at 85
C. The molds and
acrylate binders were removed by pyrolysis, followed by HA green body sintering. With this
method, implants with six different channel designs were built successfully and the designed
channels were reproduced in the sintered HA implants. The channels created in the sintered
HA implants were between 366 mm and 968 mm in diameter with standard deviations of 50 mm
or less. The porosity created by the channels were between 26% and 52%. The results show
that HA implants with designed connection pattern and well controled channel size can be
built with the technique developed in this study.
# 2001 Kluwer Academic Publishers
Hydroxyapatite (HA) is a calcium phosphate that makes
up the majority of the inorganic component of human
bones and teeth. HA prepared in porous blocks or
granules has been studied extensively as a bone graft
material [1, 2]. The compatibility of these porous HA
implants with bone tissues has been demonstrated in
several researches [3±7]. Several manufacturing tech-
niques have been developed for making these porous
HAs. Two methods are most widely used. The ®rst
method was developed by Roy and Linnehan by using a
hydrothermal exchange process to derive porous HA
from reef building corals . The calcium carbonate in
the coral exoskeleton is converted into HA with the
structural pattern of the coral exoskeleton preserved. The
connecting channels in the ®nal HA implants are
provided by the natural coral exoskeleton architecture.
Implants of this type have been studied extensively [3±
5, 7, 9, 10]. A second method of making porous HA
involves embedding organic particles, such as polyvinyl
butyral [11, 12], naphthalene , and acrylic beads 
in HA powder. HA powder is dry-pressed along with the
organic particles. At high temperature, the organic
particles are pyrolyzed, leaving pores in the size range
of the original particle. The green body is then sintered
into ceramics. In both processes, the control over the
internal porous structure of the implants is very minimal.
Undesirable isolated pores and blind ends are common in
implants manufactured with the organic particle tech-
nique . The coralline HA only contains the porous
structure provided by the exoskeleton pattern of the
harvested coral. The hydrothermal exchange process
does not offer any control over the porous structure.
In this research, we have explored a new technique of
manufacturing porous HA implants with designed
channel pattern. This process is essentially a lost-mold
shape forming process involving the use of
StereoLithography (SL) and a highly loaded ``reactive
ceramic suspension''. SL is a technique capable of taking
the 3D computer scanning image or the computer design
of an object and constructs a three-dimensional repre-
sentation of the object from epoxy resin . Several
0957±4530 # 2001 Kluwer Academic Publishers 471
researchers have demonstrated the versatility of this
technology in making complicate-geometry objects like
surgical models [16±19]. ``Reactive ceramic suspen-
sion'' refers to a ceramic suspension with ceramic
powder dispersed in a reactive medium that can be
polymerized or cured by heat or radiation. Ceramic
suspensions like these have been used to make net-shape
ceramics. Venkataswamy et al.  dispersed ceramic
powders in acrylate monomers, which were later injected
into molds and cured by heat. The cured suspension was
removed from the mold and the acrylate binder was
pyrolyzed, followed by sintering of the green bodies into
ceramics. Similarly, Janney  dispersed ceramic
powders in trimethylol propane triacrylate and hexane-
diol diacrylates. The suspensions were polymerized by a
free-radical thermal initiator. The binder-removal and
sintering process were similar to what was described
above. Young et al.  developed an aqueous ceramic
suspension by dispersing alumina powder in acrylamide
(AM) and N, NH
Ceramic objects with complicated shapes were made
with this aqueous ceramic suspension.
In this investigation, a highly loaded HA-acrylate
suspension was developed and characterized. Epoxy
molds with designed interconnected beams and channels
were made with an SL apparatus (SLA-25O, 3D
Systems, Valencia, CA). HA suspension was cast into
the molds and was thermally cured. The epoxy molds and
the interconnected beams were removed by pyrolysis to
create the channel space in the implants. The acrylic
binders in the cured HA suspensions were removed at the
same time with the epoxy molds. Upon sintering, the
pore channels left by the epoxy beams were preserved
and the hydroxyapatite green body was densi®ed to solid
beams. The channel size, wall size, and the total porosity
of the ®nal implants were characterized. The overall
process is illustrated in Fig. 1.
2. Experimental Procedures
2.1. Powder characterization
Commercial hydroxapatite (HA) powder (Plasma Biotal
Limited, North Derbyshire, UK) was used in this study.
Under the scanning electron microscope (SEM), the
powder was needle-shaped with about 60 nm in diameter
and 600 nm in length. The density of the powder was
measured with a He pycnometer (AccuPyc 1330,
Micromeritics Instrument Corp., Norcross, GA) to be
. To assess the powder sinterability, cylind-
rical pellets of 12.7 mm in diameter and 4 mm in height
were made by dry-pressing the HA powder at 34.5 MPa
(5000 psi) in a stainless steel cylindrical die. These dry-
pressed pellets were sintered in air at 800
C and 1350
C with a
sintering rate of 10
C/min. After sintering, the apparent
density of each group was measured. The phase purity of
the as-received powder and the sintered specimens were
investigated with an X-ray diffractometer (XRD,
Rota¯ex, Rigaku, Tokyo, Japan). The samples were
scanned from a 2 theta angle of 2
with a scanning
speed of 2 /min. The as-received powder and the 1350
sample were also analyzed with a diffuse re¯ectance
infra-red spectrophotometer (Galaxy 3020, Mattson
Instrument Inc. Madison, WI) at a resolution of 4 cmÀ 1
with wave number from 400 to 3000 cmÀ 1
2.2. Suspension preparation, curing and
A mixture of 50 wt % propoxylated neopentoglycol
diacrylate (PNPGDA) and 50 wt % isobornyl acrylate
(IBA) was used as a suspension vehicle. To determine the
optimal dispersant concentration, a 12 vol % HA/
PNPGDA/IBA suspension was ®rst prepared. A 1 : 1
mixture of quaternary ammonium acetate*
was used as a dispersant for the ceramic
powder. The dispersant was added to the 12 vol %
Figure 1 Flow chart of HA implant manufacturing process.
Emcol CC-55, Witco Corp. Houston, TX.
Emphos CS-1361, Witco Corp. Houston, TX.
HA/PNPGDA/IBA suspension at 1% to 6% to the dry
ceramic powder weight. The viscosity of the suspension
at each dispersant dose level was measured with a Bohlin
Rheometer (Bohlin CS-50, Bohlin Instruments,
Cranbury, NJ). The dispersant dose yielding the lowest
viscosity was used for the rest of the study.
To investigate the effect of solids loading to the
viscosity of the suspension, 5±40 vol % HA suspensions
were prepared. This was done by incrementally adding
the HA powder to the PNPGDA/IBA premix along with
the experimentally determined dispersant dose, followed
by vigorous mixing. The viscosity of the suspension at
different solids loading was measured with a Bohlin
Rheometer with a shear rate of between 0:01 sÀ 1
1000 sÀ 1
A thermal curing mechanism was used to solidify the
40 vol % HA suspension, using Benzoyl Peroxide (BPO)
at 0.15% to the monomer weight as a thermal initiator.
The BPO decomposes upon heating, releasing free
radicals that initiate the polymerization reaction of the
PNPGDA/IBA monomers. A detailed analysis of
acrylate curing is presented elsewhere . To investi-
gate the effect of the binders to the ®nal phase purity of
the ceramic, sintered samples prepared from the cured
suspensions were analyzed with XRD. HA suspension
was ®rst cured in 14 ml glass vials at 85
C for 1 h.
The samples were removed from the glass vials and
heated at a heating rate of 0.3
C/min from room
temperature to 550
C to remove the acrylate binders.
After binder removal, green bodies were sintered at
C. The phase purity of each specimen was again
investigated by XRD. The amount of residual carbon in
C specimen was analyzed with carbon
coulometry at the Department of Geological Sciences
at the University of Michigan. In carbon coulometry, a
sintered HA specimen was combusted in a combustion
apparatus and the amount of residual carbon was
determined by the amount of CO2 formed during
2.3. Implant design, manufacturing and
Six tetragonal and cylindrical implants were designed.
All implant designs are illustrated in Fig. 2a±d and the
names and dimensions of these designs are summarized
in Table I. The tetragonal prototype implants were
designed with a commercial CAD software (Unigraphics
V.11) on a Silicon Graphics Workstation. Square
channels separated at equal distances were allowed to
intersect vertically in X, Y, Z directions and penetrate
throughout the tetragonal block. The cylindrical proto-
type implants were generated from an image
manipulation process previously described . In the
cylindrical designs, C1 has channels intersecting in X, Y
directions only and C2 has channels in all X, Y and Z
directions. C3 design has a central column running in Z
direction with channels extending from the center toward
outside surface in radial directions. The negative images
of the implant designs are shown in Fig. 2e±h to reveal
the designed channel patterns inside the implants. These
negative images were used to manufacture the molds on
the Stereolithography apparatus with a commercial
Before casting, the molds were cleaned with iso-
propanol alcohol. BPO initiator was mixed into the
40 vol % HA suspension just prior to casting. Vacuum
was applied to the suspension to remove the entrapped air
during suspension preparation. The 40 vol % HA/
PNPGDA/IBA suspension was cast at room temperature
Figure 2 Implant designs (a) T1, T2 and T3 design, (b) C1 design, (c)
C2 design, (d) C3 design, (e) negative image of T1, T2, T3 designs, (f )±
(h) negative images of C1±C3 designs.
Cibatool SL5170, 3D Systems, Valencia, CA.
into the epoxy molds and cured at 85
C for 1 h. The
epoxy molds and the cured acrylic binders were
pyrolyzed in an ashing furnace with a heating rate of
C/min from room temperature to 550
C. The green
bodies were sintered at 1350
C with a heating rate of
C/min. Sintered HA implants were observed under
optical and electron microscopes. The overall dimen-
sions, channel size and wall size were measured under an
optical microscope. The implant porosity was calculated
from the weight and the overall volume of the implant.
In this paper, ``implant porosity'' is used to describe
the percentage of macroscopic void space in the
implant resulting from the built-in channels. ``Sintering
porosity'' is used to describe the percentage of
microscopic voids left within the HA structure after the
HA powder has gone through the sintering process.
3.1. Powder characterization
Fig. 3 shows the sintered density versus temperature of
the dry pressed pellet. The ®nal density of the specimens
sintered at 800 to 1350
C was found to increase from
55% to 95% of the theoretical density. Sintered density of
95% occurred at l290 to l350
C. The powder retained
HA structure from room temperature up to 1350
without formation of any second phase detectable by
XRD. The as-received powder was found to have IR
peaks similar to the results described by Fowler . The
spectra shown in Fig. 4, had bands which were identi®ed
as followed: a n4PO4 peak at 570 cmÀ 1
, a smaller OH
liberation peak at 650 cmÀ 1
, a weak n1PO4 peak at
960 cmÀ 1
, and a strong n3PO4 peak in the 1050 cmÀ 1
1100 cmÀ 1
region. A small peak for OH stretching was
also) identi®ed at 3600 cmÀ 1
. In the 1350
C sample, an
additional peak was found in the 475 cmÀ 1
was assigned a Ca3-O stretching band .
3.2. Suspension preparation and
Fig. 5 shows the viscosity versus dispersant dose of the
12 vol % HA suspension. Without any dispersant added,
the 12 vol % HA suspension was pasty. After 2% of the
dispersant was added, the suspension was able to ¯ow
easily. At a dispersant dose of 3%, the suspension was
shear-thinning. When the dispersant dose was increased
to 4%, the 12 vol % suspension was apparently
Newtonian with a constant viscosity of 0.45 Pa.S. The
viscosity further decreased to 0.38 Pa.S at a dispersant
dose of 4.7% and increased to 1.00 Pa.S again at a dose of
Figure 3 Sintering curve of HA powder from 800
C to 1350
Figure 4 IR spectrum of as-received and 1350
C powder. Extra peak
was found at 475 cmÀ 1
in the 1350
TA B L E I Dimensions of the implant designs
Design shape Overall geometry Channel size (c) Wall size (w)
Tetragonal (T1) X, Y 10.8 mm 1200 mm 1200 mm
Z 3.6 mm
Tetragonal (T2) X, Y 9.0 mm 1000 mm 1000 mm
Z 3.0 mm
Tetragonal (T3) X, Y 8.1 mm 900 mm 900 mm
Z 2.7 mm
Cylindrical (C1) Diameter 8.25 mm 500 mm 800 mm
Height 10.90 mm
Cylindrical (C2) Diameter 9.49 mm 400 mm 800 mm
Height 6.01 mm
Cylindrical (C3) Diameter 9.51 mm 400 mm
Height 6.51 mm
6%. A dispersant dose of 5% was used in preparing the
5±40 vol % HA suspension. Fig. 6 shows the measured
viscosity versus the solids loading of the suspensions.
The viscosity of the suspension was found to remain
below 1 Pa.S at solid loadings lower than 30 vol %. The
viscosity increased dramatically after 30 vol % and
reached 15 Pa.S at a solid loading of 40 vol %. A detailed
analysis of the rheological behavior is presented else-
With BPO added, the 40 vol % HA suspension cured
into solid at 85
C in less than an hour. After removing
the epoxy mold and the acrylate binders, less than 0.5%
of the residual carbon was found in the remaining HA
green structure, as determined by carbon coulometer.
Fig. 7 shows the XRD pattern of samples after sintering
at 800 to 1350
C. No second phase was detected in these
sintered samples prepared from the cured suspensions.
Fig. 8 shows the as-®red structure of the HA sample
after sintering at 1350
C for 1 h. The sintered HA
microstructure was quite dense with * 4 mm equiaxial
3.3. Implant design, manufacturing and
The suspensions ®lled up the mold during casting
without any dif®culty. After curing at 85
C for one
hour, several cured specimens were sectioned and
examined. As shown in Fig. 9, no uncured suspension
or empty voids were observed in the sectioned samples.
After binder burnout and sintering, all of the HA
implants came out successfully and were found to
preserve the overall shape and designed channel patterns.
Fig. 10 shows the sintered HA samples from all six
designs. Several SEM pictures of the implants are shown
in Fig. 11. Fig. 11 (a) shows the external surface of a C1
implant with top surface fractured to show the channels.
Well-de®ned channel shape can be seen on the surface.
Figure 6 Viscosity of 5±40 vol % HA/PNPGDA/IBA suspension with
Figure 7 XRD pattern of as-received HA powder and specimens
prepared from HA suspensions after curing at 85
C and sintered at
C to 1350
C. * indicates HA peak.
Figure 8 SEM micrograph of sintered HA showing densely sintered
structure without open pores.
Figure 5 Viscosity of 12 vol% HA/PNPGDA/IBA suspension, with a
1 : 1 mixture of quarternary ammonium acetate and aromatic phosphate
ester as the dispersant.
Fig. 11(b) shows the cross-section through the center
column of a C3 implant, the center column to the left and
the external surface to the right. Straight channels can be
seen to connect the center column with the external
surface. Fig. 11(c) shows the external surface of a C3
implant. The channels were found to exit the implant in a
To check the uniformity of the sintering shrinkage, the
dimensions of T1, T2, T3 and C1 were measured in
several locations. The results are shown in Table II. The
linear sintering shrinkage of these HA implants was
found to fall in a small range between 25 and 27% with
an average of 26+0:6%. The result indicates an even
sintering shrinkage in the measured directions. Z
direction in the tetragonal implants was not measures
due to some material loss during sample polishing. To
compensate for the shrinkage, the negative mold designs
of C2 and C3 were expanded with a shrinkage factor of
1.37 before manufacturing on the SL apparatus. The
molds were manufactured, cast and cured and the green
bodies were sintered as previously described. Table III
shows actual sintered diameter for C2 and C3. The
difference between the design dimension and the sintered
dimension reduced from 26% to 2% after the imple-
mentation of the shrinkage factor.
Table IV shows the range of channel size in all six
designs. The average channel sizes in the tetragonal
implants were between 693 and 968 mm. The average
channel sizes in the cylindrical implants were between
366 and 444 mm. The later channel sizes are well in the
range where most bone ingrowth was found [3, 9, 28, 29].
The standard deviations of the channel size in all designs
are 50 mm or less. With different channel connection
patterns, implant porosity between 26% and 52% was
The sintering of Biotal HA powder has been studied by
Ruys et al. . The powder was found to exhibit a
sigmoid sintering curve in the temperature-density data,
with a plateau in the 1100
C to 1350
C range. The ®nal
sintered density was found to be between 81% and 99%.
The shape of our temperature-density curve was similar
to this research but with a plateau occurred at a higher
temperature. The temperature for the plateau is known to
Figure 9 Cross-section of cured HA suspension inside the epoxy mold.
Figure 10 Sintered HA implants: (a) T1, T2, T3 design; (b) C1 design;
(c) C2 design; (d) C3 design.
be a function of particle size and shape and may vary
from batch to batch .
It is known that that dehydroxylation in HA can occur
without losing the HA structure when the mineral was
heated at temperatures of 800
C and above . Elliott
 has reviewed the IR spectrum study on the
dehydroxylated HA, or oxyhydroxyapatite (OHA). The
researcher concluded that the IR spectrum of OHA
contains two additional principal peaks in the
500 to 400 cmÀ 1
region ( * 475, *433 cmÀ 1
compared with HA. The additional peak found in the 475
region was proposed to be a Ca3-O stretching band
resulted from the dehydroxylation. The 475 cmÀ 1
peak in the IR result of our sintered specimen indicates an
OHA formation in our ®nal sintered implant. Ducheyne
et al. found that OHA has an aqueous solubility between
stoichiometric HA and b-Tricalcium phosphate (b-TCP)
. OHA is known to take up carbonate groups when
submerged in simulated physiologic solutions . The
formation of carbonate-containing apatite on the surface
of calcium phosphate ceramics may be an important step
leading to bonding with bone .
In the process developed in this study, the molds were
made by one of the most popular rapid prototyping
techniques, StereoLithography . The 40% HA
suspension was found to ®ll up the 800 mm to 1200 mm
space within the molds and solidi®ed in a convenient
curing time of 1 h at 85
C. The organic binder was found
to leave a small amount of residuals after binder burnout,
which greatly reduced the possibility of adverse tissue
response from the organic component of the suspension.
The solid portions of the implant were composed of
densely sintered hydroxyapatite which endow the
implant with suf®cient mechanical integrity to withstand
future handling. The designed channel space and
connection patterns were preserved during and after
sintering. Since the 40 vol % HA suspension has a
uniform sintering shrinkage of 26%, the shrinkage can
be conveniently compensated by expanding the CAD
design of the epoxy mold with appropriate shrinkage
factor. As demonstrated in this investigation, the
dimensional error between the designed value and the
actual sintered implant was reduced to 2% by just one
The dimensional resolution of this process is of
interest because it can determine the ®nest channel size
achievable in the implant. In this study, the ®nest channel
size achieved was about 366 mm. This, however, does not
represent the lower limit of this process. The channels in
the ®nal HA implants are originally occupied by epoxy
beams in the molds. The minimum size of the epoxy
beams cured by the UV laser on SLA machine actually
Figure 11 SEM pictures of sintered implants: (a) External surface of
C1 implant with top surface fractured. The channel size and shape are
well de®ned. (b) Vertically fractured C3 implant showing channels
going from inside vertical column (left) to out side surface (right). (c)
External surface of C3 implant showing well de®ned round channels.
TA B L E I I Final dimensions of T1, T2, T3 and C1 implants
Design Measured value*
(mm) Sintering shrinkage (%)
Tetragonal (T1) X, Y 7:91+0:13 26
Tetragonal (T2) X, Y 6:68+0:06 25
Tetragonal (T3) X, Y 5:90+0:02 27
Cylindrical (C1) Diameter 6:05+0:02 26
*Due to material lost in polishing, the Z dimensions were not measured.
determines the lower limit of the channels in the green
state. Current He-Cd laser used on SLA250 has a laser
spot size of 200 mm. This represents the lower limit of the
cured epoxy beams in the mold, which is also the lower
limit of the channel size in the implant in green state. An
even smaller channel size can be expected after sintering.
This lower limit in channel size will be utilized in future
investigations. The range of implant porosity in this
study was between 26% and 52%. We expect to create
implants with a wider porosity range in subsequent
We have successfully formulated a ¯owable 40 vol %
HA suspension appropriate for casting. Epoxy molds
designed with CAD software and CT scan images were
made on an SLA machine. A HA suspension was
successfully cast into the molds followed by binder
burnout and sintering to yield HA implants with well-
de®ned three-dimensionally interconnected channels.
Hollister et al.  have successfully demonstrated the
feasibility of using the combination of CT and CAD data
to design implants with de®ned channel patterns. Porous
HA with such characteristics can be a potential tool for
studying the effect of channel size, channel connection
pattern, and total porosity on cell ingrowth. The process
developed in this study demonstrate that these porous HA
implants with speci®c channel designs can actually be
manufactured. The in vivo and in vitro studies of these
implants are currently under investigation and will be
reported in the future.
1. L . L . H E N C H , J. Am. Ceram. Soc. 81 (1998) 1705.
2. E . S H O R S and R . H O L M E S , in ``An Introduction to
Bioceramics'' edited by L . L . H E N C H and J . W I L S O N (World
Scienti®c, Singapore, 1993) p. 181.
3. M . E L D E E B and R . H O L M E S , J. Oral Maxillofac. Surg. 47
4. R . E . H O L M E S , Plast. Reconstruct. Surg. 63 (1979) 626.
5. R . H O L M E S , V. M O O N E Y, R . B U C H O L Z and A . T E N C E R ,
Clin. Orthoped. 188 (1983) 252.
6. C . A . VA N B L I T T E R S W I J K , J . J . G ROT E , W. K U I J P E R S , W. T.
D A E M S and K . D E G RO OT, Biomaterials 7 (1986) 137.
7. R . A . AY E R S , S . J . S I M S K E , C . R . N U N E S and L . M .
WO L FO R D , J. Oral Maxillofac. Surg. 56 (1998) 1297.
8. D . M . ROY and S . K . L I N N E H A N , Nature 247 (1974) 220.
9. J . - H . K UÈ H N E , R . B A R T L , B . F R I S C H , C . H A M M E R , V.
J A N S S O N and M . Z I M M E R , Acta Orthop. Scand. 65 (1994) 246.
10. U . R I PA M O N T I , S . M A and A . R E D D I , Matrix 12 (1992) 202.
11. D . - M . L I U , Ceram. Int. 23 (1997) 135.
12. Idem., J. Mater. Sci. Lett. 15 (1996) 419.
13. J . B O U L E R , M . T R E CA N T, J . D E L E C R I N , J . ROY E R , N .
PA S S U T I and G . D AC U L S I , J. Biomed. Mater. Res. 32 (1996)
14. E . T S U R U G A , H . TA K I TA , H . I TO H , Y. WA K I S A K A and Y.
K U B O K I , J. Biochem. 121 (1997) 317.
15. R . F E D C H E N KO , in ``Stereolithography and other RPM
Technologies'', edited by P. Jacobs (ASME Press, Dearborn,
MI, 1996) p. 2.
16. H . A N D E R I , D . Z U R N E D D E N , W. M U H L B A U E R , K .
T W E R DY, E . Z A N O N , K . W I C K E and R . K N A P P, Brit. J.
Plast. Surg. 47 (1994) 60.
17. T. B A R K E R , W. E A R WA K E R , N . F RO S T and G . WA K E L E Y,
Aust. Phys. Sci. Med. 16 (1993) 79.
18. N . M A N KOV I C H , A . C H E E S E M A N and N . S TO K E R , J. Digital
Imaging 3 (1990) 200.
19. H . K L E I N , W. S C H N E I D E R , G . A L Z E N , E . VOY and R .
G U N T H E R , Pediatr. Radiol. 22 (1992) 458.
20. K . V E N K ATA S WA M Y, R . WA AC K , B . N OV I C H and J .
H A L LO R A N , (1990) U.S. Patent 4,978,643.
21. M . A . J A N N E Y, (1990) U.S. Patent 4,894,194.
22. A . C . YO U N G , O . O . O M AT E T E , M . A . J A N N E Y and P. A .
M E N C H H O F E R , J. Am. Ceram. Soc. 74 (1991) 612.
23. T. - M . G . C H U and J . H A L LO R A N , J. Am. Ceram. Soc. 83 (2000)
24. S . H O L L I S T E R , T. M . C H U , R . E . G U L D B E R G , P. K . Z Y S S E T,
R . A . L E V Y, J . W. H A L LO R A N and S . E . F E I N B E R G , in
``IUTAM Synthesis in Biosolid Mechanics'', edited by P.
P E D E R S E N and M . B E N D S O E (Kluwer Press, 1998) in press.
25. B . FOW L E R , Inorg. Chem. 13 (1974) 194.
26. J . E L L I OT T, in ``Structure and Chemistry of the Apatites and
Other Calcium Orthophosphates'', edited by J . E L L I OT T,
(Elsevier, New York, 1994) p. 179.
27. T. - M . G . C H U and J . H A L LO R A N , J. Am. Ceram. Soc. 83 (2000)
28. G . D AC U L S I and N . PA S S U T I , Biomaterials 11 (1990) 86.
29. O . G A U T H I E R , J . B O U L E R , E . A G U A D O , P. P I L E T, and G .
D AC U L S I , ibid. 19 (1998) 133.
30. A . R U Y S , M . W E I , C . S O R R E L L , M . D I C K S O N , A .
B R A N D WO O D and B . M I LT H O R P E , ibid. 16 (1995) 409.
31. A . R U Y S , C . S O R R E L L , A . B R A N D WO O D and B .
M I LT H O R P E , J. Mater. Sci. Lett. 14 (1995) 744.
32. T. K I J I M A and M . T S U T S U M I , J. Am. Ceram. Soc. 62 (1979)
33. P. D U C H E Y N E , S . R A D I N and L . K I N G , J. Biomed. Mater. Res.
27 (1993) 25.
34. S . R . R A D I N and P. D U C H E Y N E , ibid. 27 (1993) 35.
35. M . J A R C H O , Clin. Orthoped. 157 (1981) 259.
Received 8 June
and accepted 14 December 1999
TA B L E I I I Final dimensions of C2 and C3 design. A shrinkage factor was introduced in the dimensions of the molds of these two designs
Design Measured value*
(mm) Per cent error from original design
Cylindrical (C2) Diameter 9:26+0:08 2
Cylindrical (C3) Diameter 9:31+0:04 2
*Due to material lost in polishing, the Z dimensions were not measured.
TA B L E I V Channel size, wall size and implant porosity of the sintered HA implants
Design shape Channel size (mm) Wall size (mm) Implant porosity (%)
Tetragonal (T1) 968+45 755+48 52
Tetragonal (T2) 763+50 693+32 47
Tetragonal (T3) 693+17 631+37 48
Cylindrical (C1) 420+24 560+35 26
Cylindrical (C2) 444+26 748+17 44
Cylindrical (C3) 366+36 38